Study of microstructure of chill cast aluminium br onzes (Cu-A l-Fe-Mn)
R. D. (1UPTA, D. P. CHAKRAVARTY, R. CHAKRAVARTY and P. K. GUPTE
SUBSTANTIAL information is available on the microstructures of high tensile aluminium -bronzes but most of the literature is pertaining to the alloys containing nickel. Exhaustive amount of work was carried out by Gupta et al. at the National Metal- lurgical Laboratory to study the mechanical proper- ties of aluminium-bronze alloys in the chill-cast condi- tion without nickel addition, the results of' which have already been reported in an earlier paper.' The present paper relates to the study of microstructures of these chill-cast aluminium-bronze alloys. A few microstruc- tures of Cu-Al-Fe system have been given by Copper Development Association in their recent publication on aluminium -bronzes.2
The microstructures studied earlier were at low magnification and did not appear to have any effect on the proof stress values of these alloys. In the present work an exhaustive study was undertaken on the microstructures of more than hundred alloys, to find out whether there is any relation of the micros- tructure to the proof stress and elongation values of the alloys. Different etching reagents have been used to have a proper evaluation of the structures. The bronzes which are under study contain 8,8 to 10.8 %o aluminium , with additions of 2 to 6.0 per cent iron, 0'01 to 3.4 per cent manganese and balance copper.
All these alloys exhibited minimum ultimate tensile strength of 60 kg mm", proof stress between 20 and 24 kg/mm° and elongation from 10 to 50 per cent.
Based on the exhaustive .study on the production and mechanical properties of'the high tensile ahnninium-bronzes in the range of aluminium 8'5-1 0 .80;,, iron 2-60;, and manganese 0,1-5.5%, typical microstructures of a felt, compositions have been compared uvilh regard to clif%er- ent etchin t^ reagents and their mechanical properties.
minutes. The hot tops were as heavy as the castings.
During this period the cast ingot's flanges were expec- ted to have reached to a temperature of the order of 400 C to 500°C.
Effect of etching reagents
During preparation of the specimens for metallogra- phic examination it was observed that when different
The alloys were melted in different types of furnaces viz. gas and oil-fired crucible furnaces of 10-lb capa- city, indirect electric arc and direct electric arc fur- naces of 10-lb and 50-lb capacity respectively. All the alloys were cast in a specially shaped cast iron mould shown in Fig. I preheated to about 150 C, in the temperature range of 1080 C to 1 180°C. The cast- ings were immediately stripped as soon as the hot tops had solidified. The process hardly took two
Messrs R. D. Gupta. D. P. Chakravarty, R. Chakravarty and P. K. Gupte. National Metallurgical Laboratory, Jamshedpur.
I Split cast iron mould design for crucified small ingot test piece (dimensions in mm)
. -^YI^Y !^Yit
Gupta el W. : .Siu1v of nrirrovtructu c of chill ra c1 ahmrinirrm hron :e.c (Cu- .91-Fe-,1lrrl
(c) rVaOH (a) f eCln
(b) NH, (H 1/ 2 0,2 (d) fl,PO,
2 Effect a]' etching reuge ntv
etching reagents were used for the same alloys the structure appeared to he altogether different in each case . The effect of the following etchants is shown in Fig. 2.
1. Ferric chloride.
2. Ammonium hydroxide and hydrogen peroxide.
3. Sodium hydroxide (electrolytic etching).
4. Orthophosforic acid (electrolytic etching)
However, the specimens which were etched with ferric chloride after electrolytic polishing gave very clear structures.
For a systematic study the Cu-Al-Fe-Mn alloys which are represented in the paper along with their microstructures, have been grouped under the following three categories :
Category •:1' (Alu- deals with different sets of alloys, mini urn as variable) each set having the same iron and manganese percentage but different aluminium contents.
Category 'IV ( Iron deals with different sets of alloys as variable) each set having the same alu- minium and manganese percentage but different iron contents.
Category '(' (\langa- deals with different sets of alloys, nese as variable) having the sane aluminium and iron percentage but different manganese contents.
Gupta et al .: Study of microstructure of chill cast aluminum, bronzes (Cu-Al-Fe-Mn)
G co sIo ISTANCE oC. ISOLATED
VARIABLE BEHAVIOUR +SEMN CONTINUOUS
DA ST oCrCO
GOOD CORROSION RESIS
8^6 8.8 9.0 9-2
3 Influence of aluminium: content and cooling rate on the corro- sion resistance of binary copper -aluminium alloys
RESULTS and DISCUSSION Mechanical properties vs composition Aluntiniunt variable
Alloys pertaining to category A are given in Table I with their chemical composition and mechanical pro- perties (0-2% proof stress and elongation). From the table it can he seen that elongation decreases with increase in aluminium content of the alloy while in case of the proof stress no correlation can be made with the aluminium content of the alloy.
DANGEROUS STRU 31-Fe *SEMI - CONTINUOU:
!•h Fe OX
GOOD CORROSION RESISTANCE
"- 8-5 9'0
4 Effect of iron and aluminium content and cooling rate on corrosion resistance of ternary Cu-Al-Fe alloys
TABLE I Category A-Alloys with variable aluminium
Chemical composition wt % Mechanical properties
Alloy 0'2% proof
no. Al Fe Mn kg mm2 tion %
113 9-46 2'06 0'37 18.8 40
72 1005 2.1 0.59 24 26
58 10-50 1.9 0.54 21-68 24
130 10.50 2'11 0.25 23 24
73 10'70 1'85 0-63 23.68 12
100 8.8 2.7 0*45 24 40
135 9.45 2-94 0-38 22.8 37
120 9'6 4.29 0.42 23 40
129 10-20 4.22 0-24 20'5 34
5 6 7 8 9 10 II 12 13 14 15 WEIGHT PERCENTAGE ALUMINIUM 5 Vertical section of the Cu-AI-Fe system at 3 % Fe
Gupta et al. : Studs of rnicrocprmYure of chill enct aluminium hron:es Cii-Al-Fe-1fit
(a) 8.8%A1, 2'7% Fe , 0.5% Mn
(b) 10.0% Al, 2-1
0110Fe, 0.6% Mn
(c) 10'5°10, 1'9% le, 0'54, Mn
(d) 10'7%, Al, 2.0% Fe, 0-60' Mm 6 Effect of aluminium on microstructure
Alloys belonging to category B with variable iron con- tent are given in Table 11 with their chemical compo- sitions and mechanical properties. The study of elon- gation values of different sets of alloys given in the above table shows that elongation does not have a direct bearing on the iron content of these alumini- um-bronzes of the quaternary system of Cu-Al-Fe-Mn.
Proof stress also does not appear to be influenced by iron content of the alloy when varied between 2 and 6 per cent.
Alloys belonging to category C with variable manga- nese and constant aluminium and iron contents have been grouped with different aluminium and iron con- tents in Table III along with their chemical composi- 126
TABLE if Category B-Alloys with variable iron
Chemical Composition wt °„ Mechanical properties
no. Fe Al Mn ke nun= Lion %
72 2'10 105 0'59 24 26
75 -1.1 3 1000 0 - 35 24 19
101 3'30 1000 0 53 23 30
104 2'1 9'5 1'6 218 40
83 4'3 9'4 1'8 23 7 28
73 2'0 10.7 0.63 23'68 12
32 4'5 10'8 0.72 - 6
132 2'85 958 0 17 21'24 40
111 5. 1 5 ') 50 0.15 21.5 40
108 5'47 9.4 1118 21 I5 24
Gupta et al.: Study of microstructure of chill cast aluminium bronzes (Cu-Al-Fe-Mn) TABU: III Category B-Alloys u+ith variable manganese
Chemical composition wt °, o Mechanical properties
no. Mn Al Fe kglmm- tion %
93 001 1043 2'63 21.60 50
130 025 10' 51 2.11 23'00 24
106 1'75 1022 2 - 05 21'00
138 2'79 10'45 2'05 21'40 32
133 0'36 9.46 2'06 188 40
104 1,57 95 2.10 21.8 40
137 3.4 9.46 2'08 -
132 0'17 9158 2 - 85 21-4 40
136 114 9.51) 2.87 22 8 40
125 0'29 9.571 4'42 21'4 35
119 3.15 9.50 3'92 23-1 28
108 1)'18 9.49 5.42 2115 24
83 1.83 9.40 4-30 23-7 2t
tions and mechanical properties. From the table it can be observed that in alloys containing less than 10 per cent aluminium when the manganese content is increas- ed the proof stress values were found to improve with no systematic change in elongation . however, with higher aluminium above 10 per cent the effect of manganese was found to have an opposite effect i.e.
when manganese is increased from 0-25 to 2'79 the proof stress values decreased from 23-00 to 21 kgmm2 and elongation increased from 24 to 32.
In this study of mechanical properties with respect to composition it may be mentioned that the obser- vations made by Crofts3 on 3-7 per cent nickel bear- ing aluminium bronze with respect to elongation with varying aluminium and manganese percentages conform to the present work. Proof stress in alloys with less than 10 per cent aluminium with varying manganese contents showed similar trend as observed by Crofts.
Microstructure vs composition
The cooling rate in all the experimental heats had been of the same order. This critical cooling rate has been reported by Upton4 to be sufficient to prevent the transformation of 9 to a-}-y2 as this is evident from Figs. 3 and 4. Hence it has been taken for
granted that the phases that will be dealt in our investigation are limited to ., 1g and the iron-rich constituent precipitating out on cooling in the entire matrix as shown in Fig. 5.' The addition of manga- nese is not likely to produce any new phase because of its high solubility in copper except that it retards"
the breakdown of fI to 'c+y2, and even prevents this transformation when present in more than 6 per cent in the sand-cast alloys.
With increase in aluminium content the phase de- creased in amount and became finer. In case of 10'7 per cent aluminium it was in the form of needles as shown in Fig. 6 (d). The iron-rich phase became finer with increase in aluminium content except in the case 8.8 per cent aluminium (Fig. 6a) where it was in the lamellar shape which may be due to a little high iron content compared to other alloys.
In the alloys having high aluminium content above 10'5 per cent with increase in the iron content from 2 to 45 per cent, it was observed from Figs . 7a and 7b that the overall grain size was reduced considerably with increase in iron content . When aluminium con- tent was about 10 per cent, increase in iron from 2 to 3.1 per cent was having a marked effect on the structure as shown in Figs. 7c and 7d. The coarse overall grain boundary shown in alloy 72 ( Fig. 7c ) was completely absent in alloy 75 (Fig. 7d). The precipitation shown in alloy 72 is both as needle and globular and is coarse in nature ; however, with increase in iron con- tent the precipitation became finer with the needle shaped completely disappearing as in alloy 75. In alloys with less than 10 per cent aluminium similar observations were made as above in the structure when the iron content varied from 2 to 5 per cent (Figs. 8a, 8d).
With aluminium below 10 per cent and iron percentage constant at about 2 per cent, increase in manganese content from 0-35 to 3 5 per cent influenced the structure markedly as shown in Fig. 8. It can be seen that the constituent which was elongated and was of very coarse nature (Fig. 8a) changed to fine when the manganese content increased (Fig. 8c). The effect of manganese on the structure was further influenced by the iron content in the alloy. When the iron con- tent of the alloys was increased to above 4 per cent, change in the manganese content from 0-18 to 1.8 per cent changed the structure from uniform coarse to uniform fine distribution of ac and fI as shown in Figs. 8d, 8e. It may also be pointed out that the ^c phase distribution changed from coarse elongated needle type at low iron content to uniform fine distri- bution at high iron content in the alloys at constant manganese and aluminium contents (Figs. 8a, 8d).
(a) 10-7% Al, 2*0% Fe, 0-6% Mn
(b) 10'8 % Al, 4'5% Fe, 0'3% Mn
(c) 10.0% Al, 2'1% Fe. 0'6% Mn
(d)10 01^ Al, 3.1% Fe. 0.3% Mn 7 Effect of iron on microstructure x 55
Alloys having more than 10 per cent aluminium and 2 per cent iron with increase in manganese showed that needles got slightly coarser (Figs. 9a and 9b) which is contradictory to the effect of manganese mentioned in the earlier paragraph in case of bronzes containing less than 10 per cent aluminium.
Distribution of iron - rich phase
It may be interesting to note the shape and distribu- tion of iron in the alloys with different compositions.
It has been observed that in low aluminium alloys with high iron content the iron-rich phase separates out with coarse globular and irregular shape as shown in Fig. 10.
Microhardness was attempted in different phases in the alloy and in this context two alloys were selected with the following composition :
Alloy No. A Fe Mn
82 9-32 464 1.88
108 9 4 5-42 0-178
and their hardness was found as follows
Hardness value *V.P.N. (10 gm)
Position Alloy 82 Alloy 108
Matrix 113 106
Globular iron-rich phase - 186
Rosette iron-rich phase 276 -
Irregular iron-rich phase 359 358
*average of three readings.
Gupta et al : Stud) of microstructure of chill cast aluminium bronzes (Cu-Al-Fe-.Wn)
(a) 9'5% Al, 2-1% Fe, 0'4 Mn
(b) 9'5% Al, 2'1% Fe, 1.6% Mn
(e) 9'4% Al, 4.3% Fe, P8 Mn 8 Effect of manganese on microstructure with <10% Al x 5j
(c) 95% Al, 2.1% Fe, 3'4% Mn
(d) 9'5% Al, 5-1% Fe, 0'2% Mn
/a1'10S % Al, 2.1% Fe, 0.25%
9 Effect of manganese on microstructure with -- 10% Al
There is some difference in the hardness of the matrix and that of the globular and rosette iron-rich phase of the two alloys ; this may be attributed to the effect of manganese which is the major differing constant in the alloys. Some more work is needed in this line regard- ing the composition of these phases and their possible effect on the mechanical properties particularly the proof stress.
Microstructure vs mechanical properties in relation to compositional limits
A comparison of the microstructure with the mechani- cal properties has been made and it is observed that the microstructures can be classified into two distinct groups : (a) needle type where the cc gets precipitated in the form of needles in the matrix as shown in Figs.
7a and 8a and (b) needle free where needles are com- pletely absent in the matrix and -c is uniformly distri- buted as in Fig. 7d. These two types of structures are formed depending on the compositional limits primarily of aluminium and iron as shown in Table IV. Based on the above data it can be said that structures contain- ing needles of c are formed where (1) aluminium is less than 10 per cent with iron approximately 2 per cent and (2) aluminium above 10 per cent with iron above 2 per cent. On the otherhand structures free from -- shaped needles are formed where aluminium content of the alloy is less than 10 per cent in com- bination with iron more than 2 per cent. It may be interesting to note that the structures free from needle shaped -c exhibit proof stress above 21 kg, mm2 whereas the structures containing needle shaped -c give proof stress in the range of 19 to 24 kg/mm'2 depending upon the aluminium content of the alloy with higher aluminium percentage (more than 10 per cent) giving higher values. It is felt that the type and distribution of the needles affect the mechanical properties.
(b) 10.5% Al, 2 101, Fe. 2 84% Ain x55
TABLE,. IV Alloys with their chemical composition and mechanical properties for study of microstructure vs proof stress
Chemical composition wt °a Mechanical properties
Alloy stress Elonga-
no. Al Fe Mn kg' mm2 tion %
Needle shaped x
113 9 46 2.06 0.36 18.8 40
104 9,50 2.10 157 2118 40
137 9.46 2.08 3'4 - -
72 10.05 2 13 o-59 24 26
58 10 - 50 1 90 0 54 2168 -
129 10 22 4'22 0'24 21.5 30
73 1074 2,00 11.60 23.6 12
32 1080 4'5 0'72 6
130 10.51 2.11 0.25 23,00 24
Needle free a
75 10.0 3 10 035 24 19
83 9-40 4.30 118 21.7 28
108 940 5-47 018 2115 24
100 881 2-0 045 24 40
Gupta et al.: Shah of oucrostrurncre of chill cast alruniuium hron_es (Cu-AI-Fe-Mni
(a) 10.0°''0 Al. 3-11% Fe. 0.3% Aln
(b) 10'7% Al, 2.0% Fe, 0.6% Mn
10 Shape and distribution of iron with chemical composition x 760
The structures obtained in the chill-cast nickel-free aluminium-bronze alloys can be broadly classified into two types (a) Needle shaped -c in the matrix and (b) Structure free from -c needles.
Structure with needle shaped x is formed (a) when aluminium is less than 10 per cent with iron approxi- mately 2 per cent and (b) when aluminium is above 10 per cent with iron 2 per cent and above. Structure free from cc needles are formed when aluminium con- tent of the alloy is less than 10 per cent in combina- tion with iron more than 2 per cent.
Needle shaped ac gave high proof stress values in alloys containing more than 10 per cent aluminium.
Alloys with needle free -c also showed improvement in proof stress.
(c) 9.5% Al, 2.1% Fe, 0'4% Mn
(d 9.5% Al, 5'2% Fe, 0'2% Mn
1. Gupta, R. D., Gupte, P. K., Nijhawan , B. R. : `Studies on High Tensile Aluminium- Bronzes' presented at 35th Inter- national Foundry Congress at Tokyo in October, 1968.
2. Copper Development Association, 'The Aluminium- Bronzes' 1966. Publication No. 31. p. 202.
3. Crofts, W. L. J. : 'The Influence of Aluminium, Iron, Nickel and Manganese on Tensile Properties of Complex Alumi- nium-Bronzes'. The Journal of Australian Institute of Metals 1965, 10 (2). May. p. 149.
4. Upton, B. : 'The Corrosion Resistance in seawater on Medium Strength Aluminium Bronzes', Corrosion 1963, 19, June. 6 (C. D. A. Publication No. 31. 1966, p. 112).
S. Yutaka, A. : 'The Equilibrium Diagram of Iron-bearing Aluminium-Bronze', Nippon Kinzoku Gakkai- Si, 1941, 5 (4), p. 136 (C. D. A. Publication No. 31, 1966, p. 200).
6. Copper Development Association : 'The Aluminium- Bronze', Publication No. 31, 1966, p. 115.
Gupta et al. : Study of microstructure of chill cast aluminium bronzes (Cu-Al-Fe-Mn)
Mr A. K . Banerji (Chittaranjan Locomotive Works, Chittaranjan ) : Were the test pieces casting variables taken into consideration while studying the relationship between mechanical properties and composition?
I would also like to know the type of test pieces used, whether they were of the same composition and how many of them were used to obtain the results reported in the paper.
Dr S. S. Bhatnagar (N M L) : Did you come across martensite while examining the microstructure'?
Mr R. D. Gupta (Author) : In all the cases the mould temperature was kept at about 150 C prior to pouring as indicated in the paper.
The test pieces were machined from the flanges of the castings, as shown in Fig. I, in accordance with Indian Standard Specification No. 497 1853. The results given in the paper are the average of 3 to 4 heats of the same composition.
In answer to Dr Bhatnagar, in our range of com- position we did not notice any martensite during the investigation.